(77a) Fluidization of Graphene Nanoplatelets: From Microstructure to Hydrodynamics
The number of layers of graphene determines its microstructure which affects the powder bulk behaviour (e.g., flowability, dispersibility, fluidizability and agglomerability). One of the most interesting applications of graphene is its use in composite materials and, for example, graphene powders are emerging in the field of catalysis as excellent support materials. An attractive route for the functionalization of graphene with metal and metal-oxide nanoparticle catalysts is atomic layer deposition carried out in a fluidized bed reactor. In order to achieve an uniform deposition of nanoparticles for high-performance catalysts, ensuring a good fluidization behaviour of graphene powders is crucial. Therefore, understanding how graphene powders fluidize depending on their microstructure is vital.
In this work, we study for the first time the fluidization behavior of three kinds of graphene powders: graphene nanoplatelets of 150 m2/g (GNP150), graphene nanoplatelet aggregates of 300 m2/g (GNPA300) and graphene nanoplatelet aggregates of 750 m2/g (GNPA750). Graphene powders fall under group C of Geldartâs classification, i.e., cohesive powders. Therefore, their fluidization is expected to be prevented by the strong interparticle forces, which exceed the drag force induced by the gas flow. However, the graphene platelets do not fluidize individually, instead they form into agglomerates, due to the aforementioned cohesive forces, as earlier observed for semi-spherical nanoparticles [5, 6]. As a result, the fluidization behavior depends on the properties of the agglomerates. We correlate the morphology of the graphene nanoplatelets at nano-, micro- and macro-scales to their hydrodynamic behaviour.
GNP150 at the nanoscale consist of agglomerates of mostly 2D flakes (6-8 nm thick and 15 Î¼m wide). The latter, in virtue of being relatively thick, tend to be rigid, or in other words they are not prone to fold and wrinkle. As such, they truly enjoy a 2D geometry. Rigid 2D-like objects pack poorly compared to 3D-like flexible objects. As a result of that, agglomerates consisting of 2D thick nanoplatelets are loosely packed, hence GNP150 have a low bulk density. At the macroscale, GNP150 form mm-sized spherical agglomerates, whose size distribution depends on the history of the powder. Upon vibration-assisted fluidization, the bed of particles segregates into mm-sized agglomerates at the bottom, increasingly smaller agglomerates along the bed height, and fines above the splash zone. No fluidization is observed without the use of vibration at any of the tested superficial velocities (i.e., up to 16.85 cm/s). The use of vibration results into bubbling fluidization at relatively low superficial velocities (1.35 cm/s).
GNPA300 and GNPA750 at the nanoscale are not found in 2D form. In fact, higher-surface-area graphene powder translates into thinner nanoplatelets that are more prone to fold and wrinkle. As a result of that, the nanoplatelets are closely packed, and thus have an higher bulk density. At the macroscale, the powders look very fine and the size of the agglomerates is hardly discernable by naked eye. For GNPA300, fluidization occurs only when assisted via vibration. Fluidization occurs at higher gas velocities than in the previous case, i.e., 2.7 cm/s. Once fluidization occurs, the bed height remains approximately constant with increasing gas velocity. High superficial velocities result in slugging behaviour and significant elutriation. Instead, for GNPA750, fluidization does occur even without the use of assisting methods upon breaking of channels. In fact, increasingly thinner nanoplatelets translate into more cohesive agglomerates and higher agglomerate density. Even though cohesiveness deteriorates fluidization quality, higher densities promote fluidization. In light of this, the fact that GNPA750 fluidizes even without vibration is no surprise, as we expect the increased cohesiveness between nanoplatelets to result into highly packed and thus dense agglomerates that act as micron-sized Geldart-B-like powders.
This work demonstrates the large influence of the structure at the nm- to mm-scale on the large-scale fluidization behaviour. Such insight is essential when scaling up processes for gas-phase production of nanostructured materials .
- Lee, C., X. Wei, J.W. Kysar, and J. Hone, Measurement of the Elastic Properties and Intrinsic Strength of Monolayer Graphene. Science, 2008. 321(5887): p. 385-388.
- Balandin, A.A., S. Ghosh, W. Bao, I. Calizo, D. Teweldebrhan, F. Miao, and C.N. Lau, Superior Thermal Conductivity of Single-Layer Graphene. Nano Letters, 2008. 8(3): p. 902-907.
- Bolotin, K.I., K.J. Sikes, Z. Jiang, M. Klima, G. Fudenberg, J. Hone, P. Kim, and H.L. Stormer, Ultrahigh electron mobility in suspended graphene. Solid State Communications, 2008. 146(9): p. 351-355.
- Nair, R.R., P. Blake, A.N. Grigorenko, K.S. Novoselov, T.J. Booth, T. Stauber, N.M.R. Peres, and A.K. Geim, Fine Structure Constant Defines Visual Transparency of Graphene. Science, 2008. 320(5881): p. 1308-1308.
- van Ommen, J.R., J.M. Valverde, and R. Pfeffer, Fluidization of nanopowders: a review. Journal of Nanoparticle Research, 2012. 14(3): p. 1-29.
- Yao, W., G. Guangsheng, W. Fei, and W. Jun, Fluidization and agglomerate structure of SiO2 nanoparticles. Powder Technology, 2002. 124(1): p. 152-159.
- Salameh, S., J. Gómez-Hernández, A. Goulas, H. Van Bui, and J.R. van Ommen, Advances in scalable gas-phase manufacturing and processing of nanostructured solids: A review. Particuology, 2017. 30: p. 15-39.